Thermoelectric properties of boron carbide/HfB2 composites
Boron carbide/hafnium diboride composites were prepared by spark plasma sintering of a mixture of hafnium diboride and boron carbide powders. Boron carbide was prepared with a 13.3 at.% composition of carbon, known as the ideal carbon content to maximize the dimensionless figure of merit. The hafnium diboride content was varied between 0 and 20% by weight, and the effect on the thermoelectric properties was studied. Addition of HfB2 generally yielded an increase in the electrical conductivity and simultaneously a reduction in thermal conductivity, indicating it has potential as an enhancer of thermoelectric properties. However, the increase in electrical conductivity was not as large as observed in some composite systems, since HfB2 turned out to be a poor sintering additive leading to lower relative densities, and was furthermore offset by a moderate decrease in Seebeck coefficient. For future composite design, the sintering characteristics of the additives can be concluded as an important additional parameter to be taken into account. The optimal hafnium diboride content for relatively dense samples was found to be 10 wt%, resulting in an improvement in the maximum figure of merit, up to ZT = 0.20 at 730 °C.
KeywordsThermoelectric Boride Composite Spark plasma sintering
Thermoelectric energy generation is an increasingly intriguing prospect for use in producing green energy, particularly from waste heat processes . Recent discoveries of several new classes of thermoelectric materials like cage-structured PGECs (phonon glass electron crystal systems) [2, 3, 4, 5], nanostructured materials [6, 7, 8, 9, 10] and magnetic semiconductors [11, 12, 13] have incited a renewed interest in thermoelectric materials development. The performance of thermoelectric materials can be gauged by the figure of merit ZT = S 2 T/ρκ, where S, ρ, κ and T are the Seebeck coefficient, electrical resistivity, thermal conductivity and absolute temperature, respectively. A need exists for high-temperature thermoelectric materials which can be used to convert waste heat from thermal power plants, steelworks, factories, incinerators, etc. [14, 15, 16]. Boron cluster compounds are attractive candidates for this need because of their high stability and relatively high Seebeck coefficients [17, 18, 19]. They also exhibit relatively low thermal conductivity [20, 21, 22]. Several mechanisms have been proposed to explain the low thermal conductivity [23, 24]. Namely, large number of atoms in the unit cell (i.e., crystal complexity) disorder due to typical partial occupancies of atomic sites in these crystal structures, possible rattling of metal atoms in the voids among the boron cluster structure. An interesting possibility raised is the symmetry mismatch effect, where the prominent symmetry of a basic building block of the structure, the B12 icosahedron, has a mismatch with the symmetry of the structure. However, clear proof of this effect has not yet been presented . Regarding the electrical properties, boron cluster compounds in general show the variable range hopping (VRH) behavior where both the Seebeck coefficient and electrical conductivity increase with increasing temperature [18, 25]. These features are inherently desirable for thermoelectric energy generation, and particularly so for high-temperature applications. Well-known boron compounds like boron carbide [17, 26, 27, 28] have been investigated for thermoelectrics, with recent striking p, n control demonstrated in Zr-doped β-boron , YAl x B14 [30, 31, 32] and later also MgAlB14 [33, 34]. A renewed interest in RB66 [22, 35] has also arisen with large enhancements in ZT discovered for YB48  and SmB66 . The n-type counterparts to boron carbide; the rare earth borocarbonitrides [38, 39, 40, 41] are also of interest. Regarding research for application of thermoelectric borides, it is striking that manufacture and testing of thermoelectric bulk modules containing boron carbide at elevated temperatures have been carried out recently .
Previous research has shown that the performance of boron carbide is affected by the carbon content of the material [14, 24]. It has been found that the ideal carbon content for the thermoelectric figure of merit ZT is 13.3 at.% carbon . It has also been shown that the addition of some metal-borides to form a composite material can improve the figure of merit [43, 44, 45, 46]. For example, TiB2 doped into boron carbide [43, 44] and CoB and VB2 doped into YB22C2N [45, 46]. A recent review on the thermoelectric enhancement in composites has also been given . In this work, the effect of hafnium diboride doping on the thermoelectric properties of boron carbide was studied.
Spark plasma sintering (SPS) was used to prepare samples of boron carbide/hafnium diboride composite material. Polycrystalline samples of boron carbide, in the composition of B13C2, were first synthesized by the conventional solid-state reaction process. Amorphous boron (SB Boron 99.9%) and carbon (Wako 99.9%) powders were mixed, pressed using cold isostatic press (CIP) and heated up to around 1800 °C for 12 h in vacuum using an induction furnace. The resulting polycrystalline boron carbide powder was combined with HfB2 powder (Hermann Starck Co. 99.9%) in 0–20 wt% ratios. The composite powder was prepared by grinding the materials using a pestle and mortar in ethanol to promote homogeneity of the samples. The dried powder was then placed into a graphite dye and pressed for sintering. The SPS was performed in vacuum at 1750 °C for 6 min after a 10-min ramp-up process, for 10-mm-diameter samples under 50 MPa pressure.
The samples were characterized using high-resolution powder X-ray diffraction (XRD). Powder XRD measurements with CuK α radiations (Rigaku Ultima-3) were taken to confirm the sample composition.
Resistivity and Seebeck coefficient were measured simultaneously with an ULVAC ZEM-2 in the temperature range of 323–1005 K in N2 atmosphere. Specific heat and thermal diffusivity coefficients were measured by the laser flash method (ULVAC TC-7000) from 300 to 1003 K. Thermal conductivity was determined as the product of the density, specific heat and thermal diffusivity coefficient.
Results and discussion
The thermoelectric properties were measured for each sample with varying hafnium diboride composition across a temperature range, in order to determine how thermoelectric properties depend on both composition and temperature.
Figure 3 shows that the Seebeck coefficient decreases with increasing HfB2 composition. This is expected because boron carbide is being replaced by metallic HfB2 with a small Seebeck coefficient. Therefore, the overall composite material should have a lower Seebeck coefficient.
As the HfB2 content is increased, it can be observed that the relative densities monotonically significantly decrease. This indicates that hafnium diboride hinders the sintering of boron carbide. This decrease in relative density accounts for the relatively small increase in electrical conductivity with metallic additives compared to other previously composites [39, 45, 46]. Poor sintering also accounts for the peculiar composition dependence of electrical resistivity (Fig. 4). For future composite design, we can conclude that the sintering characteristics of the additives are an important additional parameter to be taken into account. Recently, data-mining/material informatics approaches have been used to search for viable thermoelectric materials . It would accelerate research if such sintering characteristics could also be incorporated as a parameter in the search for effective additives to enhance overall thermoelectric performance.
The hafnium diboride-doped samples show a more pronounced curvature than the undoped sample when compared to the straight line fit (Fig. 7). Figures 6 and 7 indicate that the addition of hafnium diboride alters the electrical conductivity dependence on the temperature such that it no longer is well described by the polaron hopping model suggested by Wood et al. . This is expected as the governing mechanism for charge carrier transport in a composite sample is more complex than that of a single material, and furthermore, the effect of the lower relative densities on the temperature dependence is not trivial. Regarding the apparent convergence of the resistivity data of all samples above 400 °C in Fig. 4, the plot above in Fig. 7 shows the differences. However, at higher temperatures, although the 15% sample is an outlier, there is a convergence tendency compared to the points below 400 °C, and this can be considered to be because the intrinsic hopping in the boron carbide material relatively becomes more active compared to the composite effect of the added metallic component and also the porosity effect of the different densities.
The ZT value was increased from 0.19 for the non-composite material to 0.20 for the 10% wt HfB2 composite at 730 °C, corresponding to an increase of 5%. This increase with HfB2 incorporation is modest. This small effect is likely originating from the relatively small increase in the electrical conductivity due to the lower relative densities. This effect is also coupled with the reduction in the Seebeck coefficient for the composite samples. It has previously been observed for VB2-seeded YB22C2N that Seebeck coefficients can increase when partial intrinsic doping assumedly occurred from heat treatment [45, 46, 47]. This effect may also impact the figure of merit of the composite and should be investigated in the future. Looking for metallic borides with better sintering properties than HfB2 as an additive to boron carbide is also worthwhile.
Conclusions and future work
The addition of hafnium diboride to boron carbide to form a composite material showed an improvement in the overall thermoelectric performance of boron carbide, in spite of the poor sintering characteristics of the additive. The measurements show that the decrease in the value of the Seebeck coefficient caused by the addition of HfB2− can be countered by the relatively larger decrease in both thermal conductivity and electrical resistivity. This is obtained despite the monotonic reduction in the relative densities of the samples with HfB2 addition which is very detrimental to electrical conductivity. A maximum ZT = 0.20 at 730 °C is obtained for HfB2 content of 10 wt%. One can expect higher ZT values for better densified composites.
For future composite design, we can conclude that the sintering characteristics of the additives are an important parameter to be taken into account. It is worth further investigating similar metallic borides albeit with better sintering effect to use in a composite. Recently, data-mining/material informatics approaches have gathered increasing interest in materials development. Herein we highlight the fact that besides intrinsic properties of each constituents, computational materials design could provide a more effective impetus to the field of thermoelectricity if computations could also take into account sintering characteristics. This would eventually optimize the search for effective additives to enhance overall thermoelectric performance.
In general, boron carbide-based materials have excellent potential as high-temperature thermoelectric materials since both the Seebeck coefficient and electrical conductivity increase with temperature while the thermal conductivity is relatively small with little temperature dependence at high temperatures [42, 53], leading to a ZT value which increases strongly with temperature. We are also planning further experiments with suitable instrumentation to measure the thermoelectric properties at higher temperatures (with better densified materials) as the ZT value is expected to still increase beyond the temperature range investigated in the present study.
J.L.I. was supported by the NNIN internship program. Support is acknowledged from “Materials Research by Information Integration” Initiative (MI2I) and JSPS KAKENHI Grant Number JP16H064xx. This work was conceived by T.M., D.P. and G.G. J.L.I. carried out the main experimental work. S.M. assisted J.L.I. with the use of synthesis and measurement apparatuses and Rietveld, and I. O. gave research advice. J.L.I. mainly wrote the initial draft of the paper with revisions being written and carried out by T.M., D.P. and G.G.
- 1.Koumoto, K., Mori, T. (eds.): Thermoelectric Nanomaterials—Materials Design and Applications, vol. 182. Springer Series in Materials Science. Springer, Heidelberg (2013)Google Scholar
- 3.Uher, C.: In: Tritt, T.M. (ed.) Semiconductors and Semimetals, vol. 69, p. 139. Academic Press, New York (2000)Google Scholar
- 6.Zhao, X.B., Ji, X.H., Zhang, Y.H., Zhu, T.J., Tu, J.P., Zhang, X.B.: Bismuth telluride nanotubes and the effects on the thermoelectric properties of nanotube-containing nanocomposites. Appl. Phys. Lett. 86, 06211 (2005)Google Scholar
- 7.Poudel, B., Hao, Q., Ma, Y., Lan, Y.C., Minnich, A., Yu, B., Yan, X., Wang, D.Z., Muto, A., Vashaee, D., Chen, X.Y., Liu, J.M., Dresselhaus, M.S., Chen, G., Ren, Z.F.: High-thermoelectric performance of nanostructured bismuth antimony telluride bulk alloys. Science 320, 634–638 (2008)CrossRefGoogle Scholar
- 18.Mori, T., Berthebaud, D., Nishimura, T., Nomura, A., Shishido, T., Nakajima, K.: Effect of Zn doping on improving crystal quality and thermoelectric properties of borosilicides. Dalton Trans. 2010, 39 (1027)Google Scholar
- 19.Mori, T.: Higher borides. In: Gschneidner Jr., K.A., Bunzli, J.-C., Pecharsky, V.K. (eds.) Handbook on the Physics and Chemistry of Rare Earths, vol. 38, pp. 105–173. Elsevier, Amsterdam (2008)Google Scholar
- 24.Mori, T.: In: Rowe, D.M. (ed.) Modules, Systems, and Applications in Thermoelectrics, p. 14. CRC Press/Taylor and Francis, London (2012)Google Scholar
- 28.Cai, K.F., Nan, C.W., Min, X.M.: The influence of silicon dopant and processing on thermoelectric properties of B4C ceramics. In: Symposium Z—Thermoelectric Materials 1998—The Next Generation, vol. 545. MRS Online Proceedings Library, Warrendale (1998)Google Scholar
- 42.Feng, B., Martin, H.-P., Börner, F.-D., Lippmann, W., Schreier, M., Vogel, K., Lenk, A., Veremchuk, I., Dannowski, M., Richter, C., Pfeiffer, P., Zikoridse, G., Lichte, H., Grin, J., Hurtado, A., Michaelis, A.: Manufacture and Testing of Thermoelectric Modules Consisting of BxC and TiOx Elements. Adv. Eng. Mater. 16, 1252–1263 (2014)CrossRefGoogle Scholar
- 43.Goto, T.: Kinzoku (in Japanese) 68, 1086 (1998).Google Scholar
- 50.Eucken, A.: Thermal conductivity of ceramic refractory materials: calculation from thermal conductivities of constituents. VDI Forschungsheft 353, 16 (1932)Google Scholar
- 51.Eucken, A.: Thermal conductivity of ceramic refractory materials; Its calculation from thermal conductivity of constituents. Ceram. Abstr. 12, 231 (1933)Google Scholar
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.